CREVICE CORROSION. CREVICE CORROSION Narrow openings, gaps, spaces, pores etc. between metal-metal components or metal-non-metal components may provoke localized corrosion. NOTE: unintentional crevices (seams, cracks etc.) can also act in the same way - PowerPoint PPT Presentation
1CREVICE CORROSION2CREVICE CORROSION
Narrow openings, gaps, spaces, pores etc. between metal-metal components or metal-non-metal components may provoke localized corrosion.
NOTE: unintentional crevices (seams, cracks etc.) can also act in the same way
Passive alloys (especially stainless steels) are more vulnerable than more active alloys.3
Crevice corrosion at a metal-to-metal crevice site formed between components of type 304 stainless steel fastener in seawater4 Crevice Corrosion occurring on a Test specimen of Type 316 SS (Stainless Steel) in Acid Condensate Zone of a Model SO2 Scrubber.
5Crevice corrosion is caused by the existence of small volumes of stagnant (corrosive) solution. Small holes, gasket surfaces, lap joints, bolt or rivet heads, nuts, washers, surface deposits all can cause C.C. (Crevice Corrosion).
Type 304 SS sheet can be cut by stretching a rubber band around it, immersing it in seawater (Fontana). The crevice between the rubber and the metal acts as the cutting zone.6MECHANISMConsider riveted metal section, immersed in aerated seawater (pH 7) e.g. stainless steelAlthough O2 within crevice is rapidly used up, corrosion continues, controlled by overall cathodic reaction outside the crevice.Tendency to build up M+ within the crevice must be balanced by -ve charge diffusing in.Some OH- diffuses in, alot of Cl- diffuses in (OH- more mobile, c.f. FONTANA* less of it).7MECHANISMOxidation: M M+ + e-Reduction: O2 + 2 H2O + 4 e- 4 OH-
*FONTANA says Cl- more mobile this is wrong.
9Most metal ions (except alkali metals) hydrolyze:M+ + H2O MOH + H+Both Cl- and H+ accelerate metal dissolution (Cl- breaks down oxide, also H+ partly responsible). NOTE: there is now the possibility for H2 evolution within the crevice . . . . maybe!NOTE: solution within crevices exposed to neutral dilute NaCl has been seen to have 3-10x [Cl-] in bulk, pH of 2-3.10Later stages
11Factors that can affect Crevice Corrosion resistance of stainless steelsGeometricalType of crevice:metal to metal nonmetal to metal Crevice gap (tightness) Crevice depthExterior to interior surface area ratio
MetallurgicalAlloy composition:major elements minor elementsimpuritiesPassive film characteristics
Electrochemical reactions:Metal dissolutionO2 reduction H2 evolution12Environmental
Bulk solution:O2 contentpHchloride leveltemperatureagitation
Mass transport, migrationDiffusion and convectionCrevice solution: hydrolysis equilibriaBiological influences13CREVICE CORROSION OF CU ALLOYS different from that of SS; attack occurs OUTSIDE the crevice Crevice corrosion of Alloy 400 (70 Ni - 30 Cu) after 45 Days in Natural Seawater
14Cathodic conditions inside crevices of Cu alloy have been inferred from observations of deposited Cu metal (where?).Differential metal-ion concentration has been invoked as the mechanism; greater concentration inside the crevice raises the potential and makes it more noble than the outside.Also, variant of the oxygen depletion mechanism has been invoked. Clearly the situation is complex.NOTE: ALL MATERIALS ARE SUSCEPTIBLE TO C.C. (CREVICE CORROSION), GIVEN NARROW CREVICES, POSSIBILITY OF CONCENTRATING IONS, DIFFERENTIAL AERATION CELLS, DIFFERENTIAL METAL CONCENTRATION CELLS, ETC.15COMBATING CREVICE CORROSION (after Fontana)
Methods and procedures for combating or minimizing crevice corrosion are as follows:Use welded butt joints instead of riveted or bolted joints in new equipment. Sound welds and complete penetration are necessary to avoid porosity and crevices on the inside (if welded only from one side).Close crevices in existing lap joints by continuous welding, caulking, or soldering.Design vessels for complete drainage; avoid sharp corners and stagnant areas. Complete draining facilitates washing and cleaning and tends to prevent solids from settling on the bottom of the vessel.16COMBATING CREVICE CORROSION (after Fontana)
Inspect equipment and remove deposits frequently.Remove solids in suspension early in the process, if possible.Remove wet packing materials during long shutdowns.Provide uniform environments, if possible, as in the case of backfilling a pipeline trench.Use "solid," nonabsorbent gaskets, such as Teflon, wherever possible.Weld instead of rolling in tubes in tube sheets.17FlLIFORM CORROSIONAlthough not immediately apparent, filiform corrosion (filamentary corrosion occurring on metal surfaces) is a special type of crevice corrosion. In most instances it occurs under protective films, and for this reason it is often referred to as underfilm corrosion.This type of corrosion is quite common; the most frequent example is the attack of enameled or lacquered surfaces of food and beverage cans that have been exposed to the atmosphere. The red-brown corrosion filaments are readily visible.18Filiform corrosion usually on metals covered with thin organic film (0.1 mm) BUT also reported for:steel;magnesium;aluminum;tin;silver;gold;phosphate;enamel;as well as with organics (lacquer, paper; seen on paper-backed Al foil, between metal and paper).19A lacquered steel can lid exhibiting filiform corrosion showing both large and small filaments partially oriented in the rolling direction of the steel sheet. Without this 10 x magnification by a light microscope, the filiforms look like fine striations or minute tentacles; (often mistaken for biologically induced corrosion).
20Attack usually occurs when relative humidity between 65 and 90%; has been seen at lower R.H. (Relative Humidity).Average filament width 0.05 - 3 mm .. depending on coating (thickness, porosity, etc.), R.H., and corrosiveness of environment (presence of SO2, H2S, etc.). Filament height 20 m. Growth rates observed between 0.01 mm/d and 0.85 mm/d.Filaments are like minute tunnels, full of corrosion products.21Liquid in head is typically acidic. . . . pH 1- 4.IN ALL CASES.... O2 (or air) and water are needed to sustain filiform corrosion indicates a form of a DIFFERENTIAL AERATION CELL.Discuss:differential aeration cellconcentration cell.22
An aside on differential aeration . . (differential) concentration cell remember example: remember Cu - alloy crevice:
Attack usually begins at imperfections in coating e.g., cuts, knicks, pores, etc.CO2 can stimulate process by dissolving in water carbonic acid.Chlorides, SO42-, S2- which can dissolve in condensing atmospheric moisture also increase attack.Optimum temperature for filiform attack between 20 & 35C.
(potential log [Cu+]) 23Effect of humidity on filiform corrosion of enameled steelRelative humidity, %Appearance 0-65No corrosion65-80Very thin filaments80-90Wide corrosion filaments 93Very wide filaments 95Mostly blisters, scattered filiform100BlistersSource: M. Van Loo, D. D. Laiderman, and R. R. Bruhn, Corrosion, 9:2 (1953).
Appearance: Schematic diagram of a corrosion filament growing on an iron surface (magnified).
24Schematic diagrams illustrating the interaction between corrosion filaments:
(a) Reflection of a corrosion filament; (b) splitting of a corrosion filament; (c) joining of corrosion filaments; (d) death trap.
Head supplied with H2O by osmosis (high concentration of Fe2+ inside) through coating and from precipitated hydroxide/oxide. Oxygen reduction creates hydroxide; precipitation creates corrosion product tail. . . . further oxidation to Fe3+ oxide etc. Hydrolysis of salts in head creates acidic conditions.
Details of mechanism not understood.e.g., why do filaments reflect off other filaments? etc.
26Filiform Corrosion on PVC-Coated Al Foil
Advancing head and cracked tail of a filiform cell.Scale: 0.125 mmGelatinous corrosion products oozing out of porous tail section.Scale: 1.25 m
27Close-up of the advancing head shown in adjacent figure. Minute cracks can be seen at the head/tail interface of a filiform corrosion cell. These cracks are entry points for water and air to provide a source of hydroxyl ions and an electrolyte. Intermediate corrosion products are just beginning to form in the head, and they undergo further reaction to form an expanded tail. The tail region is a progressive reaction zone that ultimately forms spent corrosion products. Between the head and porous end, ions gradually react with water and oxygen and are slowly transported in the direction of the tail to form final corrosion products.
Scale: 15 m
28Prevention NOT EASY....
store coated metals in dry air;use more brittle films . . . these should crack at head and destroy differential aeration;use impermeable coatings.29Pitting Corrosion30Pitting CorrosionPitting factor =
d = average penetration from weight loss; p = deepest penetration
Undercuttingpit opening usually < 1 mm.
Pits may overlap to give the appearance of rough, general wastage.PITTING: Extreme localized attack, may perforate metal sheet/plate . . . etc.
31 Pitting is an insidious and destructive form of corrosion:
difficult to detect (pits may be small on surface, but extensive below surface from undercutting; may be covered with deposit);
can cause equipment to fail (by perforation) with very little weight loss;